DOI: 10.17188/1674049
title: Materials Data on LiFeP2O7 by Materials Project

description: LiFeP2O7 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are eight inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–2.39 Å. In the second Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share a cornercorner with one FeO6 octahedra, corners with four PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 74°. There are a spread of Li–O bond distances ranging from 1.83–1.99 Å. In the third Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one FeO6 octahedra. There are a spread of Li–O bond distances ranging from 1.81–2.28 Å. In the fourth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of Li–O bond distances ranging from 1.89–2.03 Å. In the fifth Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 1.90–2.62 Å. In the sixth Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share a cornercorner with one FeO6 octahedra, corners with four PO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 53°. There are a spread of Li–O bond distances ranging from 1.84–2.12 Å. In the seventh Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.84–2.57 Å. In the eighth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.93–2.39 Å. There are eight inequivalent Fe3+ sites. In the first Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with six PO4 tetrahedra, an edgeedge with one LiO4 tetrahedra, and an edgeedge with one FeO5 trigonal bipyramid. There are a spread of Fe–O bond distances ranging from 1.91–2.20 Å. In the second Fe3+ site, Fe3+ is bonded to five O2- atoms to form FeO5 trigonal bipyramids that share corners with five PO4 tetrahedra and an edgeedge with one FeO6 octahedra. There are a spread of Fe–O bond distances ranging from 1.88–2.18 Å. In the third Fe3+ site, Fe3+ is bonded to six O2- atoms to form distorted FeO6 octahedra that share corners with two LiO4 tetrahedra, corners with four PO4 tetrahedra, an edgeedge with one FeO6 octahedra, and an edgeedge with one PO4 tetrahedra. There are a spread of Fe–O bond distances ranging from 1.95–2.25 Å. In the fourth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one FeO6 octahedra. There are a spread of Fe–O bond distances ranging from 1.96–2.19 Å. In the fifth Fe3+ site, Fe3+ is bonded to six O2- atoms to form distorted FeO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Fe–O bond distances ranging from 1.91–2.36 Å. In the sixth Fe3+ site, Fe3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Fe–O bond distances ranging from 1.96–2.14 Å. In the seventh Fe3+ site, Fe3+ is bonded to five O2- atoms to form distorted FeO5 trigonal bipyramids that share a cornercorner with one LiO4 tetrahedra, corners with five PO4 tetrahedra, and an edgeedge with one FeO6 octahedra. There are a spread of Fe–O bond distances ranging from 1.94–2.17 Å. In the eighth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one FeO5 trigonal bipyramid. There are a spread of Fe–O bond distances ranging from 1.96–2.20 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 55°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two FeO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–48°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, a cornercorner with one FeO5 trigonal bipyramid, and an edgeedge with one FeO6 octahedra. The corner-sharing octahedral tilt angles are 54°. There are a spread of P–O bond distances ranging from 1.52–1.58 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three FeO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 21–50°. There are a spread of P–O bond distances ranging from 1.52–1.63 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three FeO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 27–47°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, a cornercorner with one PO4 tetrahedra, corners with two LiO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 56°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 54°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 28°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, a cornercorner with one PO4 tetrahedra, corners with two LiO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 34°. There are a spread of P–O bond distances ranging from 1.48–1.60 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two FeO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedra tilt angles range from 50–58°. There are a spread of P–O bond distances ranging from 1.48–1.60 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two FeO6 octahedra, a cornercorner with one PO4 tetrahedra, corners with two LiO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedra tilt angles range from 54–55°. There are a spread of P–O bond distances ranging from 1.51–1.60 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three FeO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 20–48°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three FeO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 29–50°. There are a spread of P–O bond distances ranging from 1.52–1.60 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 51°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one FeO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 32°. There are a spread of P–O bond distances ranging from 1.47–1.64 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two FeO6 octahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one FeO5 trigonal bipyramid. The corner-sharing octahedra tilt angles range from 55–59°. There are a spread of P–O bond distances ranging from 1.51–1.59 Å. There are fifty-six inequivalent O2- sites. In the first O2- site, O2- is bonded in a 2-coordinate geometry to two Li1+ and one P5+ atom. In the second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Fe3+, and one P5+ atom. In the third O2- site, O2- is bonded in a distorted trigonal planar geometry to two Fe3+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the fifth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Fe3+ and one P5+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Fe3+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a distorted trigonal non-coplanar geometry to one Li1+, one Fe3+, and one P5+ atom. In the eighth O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the ninth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to two P5+ atoms. In the tenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Fe3+, and one P5+ atom. In the eleventh O2- site, O2- is bonded in a distorted trigonal planar geometry to two Fe3+ and one P5+ atom. In the twelfth O2- site, O2- is bonded in a bent 150 degrees geometry to one Fe3+ and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Fe3+, and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Fe3+, and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Fe3+, and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a bent 120 degrees geometry to one Fe3+ and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Fe3+, and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to two Fe3+ and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to two P5+ atoms. In the twentieth O2- site, O2- is bonded in a distorted trigonal planar geometry to two Li1+ and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a bent 120 degrees geometry to one Li1+ and one P5+ atom. In the twenty-second O2- site, O2- is bo